Embed Size (px)
Transcript of Articulo 3.pdf
Journal of Minerals and Materials Characterization and Engineering, 2015, 3, 15-25 Published Online January 2015 in SciRes. http://www.scirp.org/journal/jmmce http://dx.doi.org/10.4236/jmmce.2015.31003
How to cite this paper: Orozco-Gonzlez, P., et al. (2015) Nucleation of Fe-Rich Intermetallic Phases on -Al2O3 Oxide Films in Al-Si Alloys. Journal of Minerals and Materials Characterization and Engineering, 3, 15-25. http://dx.doi.org/10.4236/jmmce.2015.31003
Nucleation of Fe-Rich Intermetallic Phases on -Al2O3 Oxide Films in Al-Si Alloys Pilar Orozco-Gonzlez1*, Manuel Castro-Romn2, Simitrio Maldonado-Ruz1, Sergio Haro-Rodrguez1, Fabin Equihua-Guilln3, Rodrigo Muiz-Valdez3, Salvador Luna-lvarez3, Miguel Montoya-Dvila1, Alejandra Hernndez-Rodrguez2 1Academic Unit of Engineering, Autonomous University of Zacatecas, Zacatecas, Mxico 2CINVESTAV Saltillo, Saltillo, Mxico 3Faculty of Engineering, Autonomous University of Coahuila, Mxico Email: [email protected] Received 5 September 2014; revised 7 October 2014; accepted 14 October 2014
Copyright 2015 by authors and Scientific Research Publishing Inc. This work is licensed under the Creative Commons Attribution International License (CC BY). http://creativecommons.org/licenses/by/4.0/
Abstract Nucleation of Fe-rich intermetallic phases on -Al2O3 oxide films were analyzed in five experi-mental Al-Fe-Mn-Si alloys. In an attempt to verify the role of -Al2O3 films in nucleating Fe-rich in-termetallics, experiments have been conducted under conditions where formed in situ oxide films were present. Some Fe-rich intermetallics are observed to be related with the oxide films in the microstructure, the present results are in accordance with some research that suggest that the Fe-rich intermetallic phases nucleate upon the oxide films. The intermetallic phases and -Al2O3 films were unambiguously identified with the help of complementary techniques such as thermal analysis, SEM/EDS and X-ray diffraction.
Keywords Aluminum Alloys, Intermetallics, Nucleation, Crystal Growth, Oxide Films
1. Introduction Iron is known to be the most common and at the same time the most detrimental impurity in Al-Si alloys due to its role in the formation of brittle Fe-rich intermetallic phases that precipitate during solidification process. In
P. Orozco-Gonzlez et al.
this way, commercial Al-Si alloys always contain Fe impurities; this undesirable contamination is inevitable and cannot be economically removed from the molten aluminum, it comes either from the use of steel tools for melting and casting or from the use of scrap as the initial material.
The Fe impurities have a detrimental effect on the mechanical properties and extrusion characteristics of the Al-Si alloys. This is attributed to the formation of different Fe-containing intermetallic phases, such as -AlFeSi and -AlFeSi -. The phase is usually described as having a cubic, c-Al15(Fe,Mn)3Si2,   or hex-agonal, h-Al8Fe2Si, - crystal structure, and the phase is generally considered to be monoclinic Al5FeSi -. Techniques have to be developed to neutralize the detrimental effect of Fe impurities: 1) rapid solidi-fication; 2) manganese addition; 3) melt superheating; and 4) inclusion particles addition. The three first me-thods basically convert the crystallization of the phase to the less harmful Chinese script form, c phase  . Each one of these methods has its own advantages and limitations.
The inclusion particles addition technique is based on the work performed by Campbell and co-workers - . They have reported that the Fe-rich intermetallic phases nucleate and grow on the wetted surfaces of the oxide films, which have long been identified as cracks in the castings. Campbell et al. have further applied this nucleation mechanism to explain the cracks observed along the central axis of some Fe-rich intermetallics and for remove oxide films from the liquid aluminum. According to Cao and Campbell  , the wet side of the oxide films acts as a preferential nucleation site for Fe-rich intermetallic phases. As these particles have an in-creased sedimentation tendency, they sink to the bottom, bringing the oxide films with them.
The nucleation of Fe-intermetallic phases, such as and , was reported to be enhanced in the presence of particular inclusions added such as -Al2O3 and MgAl2O4 . Khalifa et al.  have investigated the nuclea-tion of Fe-intermetallic phases on the surface of different inclusions. They have reported that some inclusions exhibit higher potency for the nucleation of particular Fe-intermetallic phases under certain conditions and poor potency under other conditions. In general, these results showed limited effect of the inclusion particles added on the nucleation of Fe-intermetallic phases. For example, -Al2O3, which is a potent nucleant for the primary phase -Al, exhibit poor potency for the nucleation of the Fe-intermetallic phases. On the other hand, Lu and Dahle  did not find direct physical contact between Fe-rich intermetallic phases and the oxide films, thus the role of the oxide films as a heterogeneous substrate of Fe-intermetallics is uncertain.
The present work was performed to provide additional experimental information about the interaction be-tween the Fe-intermetallic phases and -Al2O3 oxide films, commonly present in Al-Si alloys, in order to clarify the role of this oxide as heterogeneous substrate for the nucleation of Fe-intermetallic phases. This aspect would aid in controlling intermetallic formation, allowing control of the microstructure of the castings and hence im-provement of the mechanical properties of the commercial Al-Si alloys. It is worth mentioning that any interme-tallic phase formation on -Al2O3 films was not investigated in this work.
2. Experimental Details 2.1. Melt Preparation The chemical composition of the alloys, determined by inductively coupled plasma emission spectroscopy (ICP), is shown in Table 1. These alloys were prepared starting from aluminum ingots of commercial purity (99.79%); the main impurities present in these ingots were: 0.14% Fe and 0.05% Si. The added alloying elements were: Fe (99.98%), Mn (99.95%), and silicon of commercial grade. The chemical composition is given in weight percen-tage unless otherwise specified.
2.2. Thermal Analysis (TA) To determine the solidification sequence and the onset reaction temperature, Tp, for the intermetallic phase for-mation (see Table 2), thermal analysis curves were obtained by employing an experimental device similar to the one used by Bckerud et al. . First, the alloy was melted and heated to 800C under ambient air conditions in a gas furnace. Subsequently, the melt was poured into a graphite cup having a wall thickness of 6 mm, which was preheated to 900C in an electric furnace; to achieve thermal equilibrium conditions, the melt was kept at 900C for 120 s in the graphite cup inside the electrical furnace. Finally, the sample was cooled down to room temperature at a rate of ~1C/s.
The alloys temperature was measured with two K-type thermocouples placed on the graphite cups lid, as shown in Figure 1. The precision of the thermocouples was assessed by measuring the melting temperature of
P. Orozco-Gonzlez et al.
Table 1. Chemical composition of the aluminum alloys.
Alloy Al Si Mn Fe Fe/Mn ratio
1 85.4 13.3 1.2 0.1 0.1
2 84.2 13.5 1.1 1.2 1.1
3 81.1 13.4 1.1 4.4 4.0
4 78.2 13.5 1.2 7.1 5.9
5 75.1 13.6 1.2 10.1 8.4
Table 2. Chemical composition and structural data of extracted intermetallic phases, determined from the results of the SEM/ EDS and XRD analyses.
Alloy Tp C
Composition from SEM/EDSa Fe/Mn Weight Ratio Formula Lattice Parameter () Al Si Fe Mn
1 610 595 sc 56.90 10.69 3.45 28.95 0.12 Al34.1FeMn8.5Si6.16 a = 12.648
2 655 640 bcc 58.20 10.24 9.77 21.80 0.45 Al12.3FeMn2.27Si2.1 a = 12.603
3 679 664 bcc 57.93 10.07 18.61 13.38 1.39 Al8.8Fe1.36MnSi1.47 a = 12.535
4 732 717 h 53.27 12.51 26.46 7.76 3.41 Al14Fe3.36MnSi3.15 a = 12.39, c = 26.203
5 745 730 h 53.98 12.71 26.92 6.38 4.22 Al17.2Fe4.15MnSi3.9 a = 12.359, c = 26.14
TpOnset temperature for the intermetallic phase formation; TsIsothermal treatment temperature. aAverage of eight SEM/EDS analyses of the ex-tracted particles, for each alloy.
Figure 1. (a) Schematic illustration of the graphite cup and lid used to carry out the thermal analysis experiments; (b) Experimental setup used for the isothermal treatments.
pure aluminum 660.4C. The temperature-time data were recorded using a 16-bit resolution Daq Temp 14A card linked to a computer.
2.3. Isothermal Treatments Based on the values of Tp obtained for the formed intermetallics (see Table 2), the alloys were subjected to an isothermal treatment at a temperature set ~15C below Tp, which is hereinafter denominated as Ts. The purpose of this isothermal treatment was to allow the intermetallic particles to grow and settle down toward the bottom of the sample. Each sample was 19 mm in diameter and 25 mm in height and was placed inside a graphite cruci-ble having a wall thickness of 3 mm. A set of five crucibles, shown in Figure 1, was heated in an electric fur-nace under ambient environment at 900C for 1800 s, subsequently cooled down to Ts at ~1C/s and then held at Ts for 15 hours. At the end of the isothermal treatment, the samples were quenched in a water bath at 25C. Due to the small size of the samples, the water quenching effectively retained the solid-liquid mic